Diaquabis{μ-1,5-bis[(pyridin-2-yl)methylidene]carbonohydrazide(1‒)}di-μ-chlorido-tetrachloridotetrazinc(II)
Seck, Thierno Moussa; Gaye, Papa Aly; Ndoye, Cheikh; Thiam, Ibrahima Elhadji; Diouf, Ousmane; Retailleau, Pascal; Gaye, Mohamed; Acta Crystallographica Section E 76 (2020) 1349–1352; doi:10.1107/S2056989020009834

data_2243507
_publ_section_title
;
 Diaquabis{\m-1,5-bis[(pyridin-2-yl)methylidene]carbonohydrazide(1--)}di-\m-chlorido-tetrachloridotetrazinc(II)
;
_journal_coeditor_code           EX2035
_journal_issue                   8
_journal_name_full               'Acta Crystallographica Section E'
_journal_page_first              1349
_journal_page_last               1352
_journal_paper_doi               10.1107/S2056989020009834
_journal_volume                  76
_journal_year                    2020
_chemical_formula_iupac          '[Zn4 (C13 H11 N6 O1)2 Cl6 (H2 O1)2]'
_chemical_formula_moiety         'C26 H26 Cl6 N12 O4 Zn4'
_chemical_formula_sum            'C26 H26 Cl6 N12 O4 Zn4'
_chemical_formula_weight         1044.77
_chemical_name_systematic
Diaquabis{\m-1,5-bis[(pyridin-2-yl)methylidene]carbonohydrazide(1-)}di-\m-chlorido-tetrachloridotetrazinc(II)
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_atom_sites_solution_hydrogens   mixed
_atom_sites_solution_primary     dual
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-2018/3
_cell_angle_alpha                94.639(3)
_cell_angle_beta                 110.091(4)
_cell_angle_gamma                97.599(3)
_cell_formula_units_Z            1
_cell_length_a                   9.2002(4)
_cell_length_b                   9.4306(4)
_cell_length_c                   11.7651(4)
_cell_measurement_reflns_used    6440
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      30.6450
_cell_measurement_theta_min      4.3120
_cell_volume                     941.46(7)
_computing_cell_refinement
;
CrysAlisPro (Rigaku OD, 2018)
;
_computing_data_collection
;
CrysAlisPro (Rigaku OD, 2018)
;
_computing_data_reduction
;
CrysAlisPro (Rigaku OD, 2018)
;
_computing_molecular_graphics
;
ORTEP-3 for Windows (Farrugia, 2012)
;
_computing_structure_refinement
;
<i>SHELXL2018/3</i> (Sheldrick, 2015b)
;
_computing_structure_solution
;
SHELXT (Sheldrick, 2015a)
;
_diffrn_ambient_temperature      293(2)
_diffrn_detector                 'HPAD Dectris Pilatus3R 200K'
_diffrn_measured_fraction_theta_full 0.994
_diffrn_measured_fraction_theta_max 0.995
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'XtaLAB AFC12 (RINC): Kappa single'
_diffrn_measurement_method       '\w scans'
_diffrn_radiation_monochromator  mirror
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0490
_diffrn_reflns_av_unetI/netI     0.0373
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            15934
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.103
_diffrn_reflns_theta_min         4.401
_diffrn_source                   'micro-focus sealed X-ray tube'
_diffrn_standards_decay_%        0.0(2)
_diffrn_standards_interval_count 0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    2.994
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.37505
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
(CrysAlisPro; Rigaku OD, 2018)
;
_exptl_crystal_colour            'pale yellow'
_exptl_crystal_density_diffrn    1.843
_exptl_crystal_description       tab
_exptl_crystal_F_000             520
_exptl_crystal_size_max          0.21
_exptl_crystal_size_mid          0.10
_exptl_crystal_size_min          0.05
_refine_diff_density_max         0.804
_refine_diff_density_min         -0.941
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.045
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     244
_refine_ls_number_reflns         4127
_refine_ls_number_restraints     2
_refine_ls_restrained_S_all      1.045
_refine_ls_R_factor_all          0.0526
_refine_ls_R_factor_gt           0.0386
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0583P)^2^+0.5038P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0950
_refine_ls_wR_factor_ref         0.1025
_reflns_number_gt                3343
_reflns_number_total             4132
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            ex2035sup1.cif
_cod_data_source_block           I
_cod_original_cell_volume        941.47(7)
_cod_database_code               2243507
_shelx_hkl_checksum              45286
_shelx_res_checksum              91025
_cod_database_fobs_code 2243507